University of Pennsylvania
Publicly Accessible Penn Dissertations
Engineering Phonon, Photon, Electron and
Plasmon interactions in Silicon - Metal
Nanocavitiies for Silicon Photonics and
University of Pennsylvania, firstname.lastname@example.org
Follow this and additional works at:http://repository.upenn.edu/edissertations
Part of theMechanics of Materials Commons
This paper is posted at ScholarlyCommons.http://repository.upenn.edu/edissertations/1576
For more information, please email@example.com.
Agarwal, Daksh, "Engineering Phonon, Photon, Electron and Plasmon interactions in Silicon - Metal Nanocavitiies for Silicon Photonics and Thermoplasmonics" (2016).Publicly Accessible Penn Dissertations. 1576.
Engineering Phonon, Photon, Electron and Plasmon interactions in
Silicon - Metal Nanocavitiies for Silicon Photonics and
ENGINEERING PHONON, PHOTON, ELECTRON AND PLASMON INTERACTIONS IN SILICON -METAL NANOCAVITIIES FOR SILICON PHOTONICS AND THERMOPLASMONICS
Ritesh Agarwal, PhD
Silicon photonics offers a cost effective solution to achieve ultrafast data processing speeds. But due to its indirect bandgap structure, making lasers from silicon is extremely difficult. Thus research has focused on nonlinear Raman processes in silicon as a method to achieve optical gain. Silicon nanowires provide an interesting platform for enhancing these nonlinearities because of their small size, geometry and relevant length scales. In the current work Raman measurements done on silicon nanowires reveal that up to twelvefold enhancement in Stokes scattering intensity and fourfold enhancement in anti Stokes scattering intensity can be attained depending on cavity structure and size, and excitation wavelength. In some cavities Stokes intensity depends on the sixth power of pump intensity, indicating extreme nonlinearity. Numerical calculations, done to understand the mechanism of these results indicate that silicon nanowires confine light to highly intense electric field modes inside the cavity which lead to stimulated Stokes and anti Stokes Raman scattering. Cavity modes can also be tuned to enhance the relative emission of either one of anti Stokes or Stokes photons which could enhance cavity cooling. These results would enable the development of smallest monolithically integratable silicon laser with extremely low lasing threshold and could lead to the
development of next generation of high speed and energy efficient processors. The intense electric field inside the nanowire could also be used to enhance the degree of plasmon excitation in metallic nanoparticles. Silicon nanowires coated with a 10 nm thick gold film lead to strong plasmon excitation in gold and high cavity absorption which enable the cavity to heat up to temperatures of 1000K at relatively low pump powers. The cavities also give the ability to measure temperature attained during plasmon excitation and control the plasmon resonance wavelength. Because of the strong heating and plasmonic effects, these cavities show enhanced evolution rates of hydrogen, a crucial industrial building block and a promising fuel, in photoreforming reactions of alcohols.
Degree Type Dissertation
Doctor of Philosophy (PhD)
Materials Science & Engineering
optics, plasmonics, semiconductor, silicon photonics
Subject Categories Mechanics of Materials
INTERACTIONS IN SILICON - METAL NANOCAVITIIES FOR SILICON
PHOTONICS AND THERMOPLASMONICS
Materials Science and Engineering
Presented to the Faculties of the University of Pennsylvania
Partial Fulfillment of the Requirements for the
Degree of Doctor of Philosophy
Supervisor of Dissertation
Ritesh Agarwal, PhD
Professor of Materials Science and Engineering
Graduate Group Chairperson
Shu Yang, PhD, Professor of Materials Science and Engineering
Nader Engheta, PhD, H. Nedwill Ramsey Professor of Electrical and Systems
Engineering, Physics and Astronomy and Materials Science and Engineering and
Christopher B. Murray, PhD, Richard Perry University Professor of Chemistry, and
Materials Science and Engineering
Cherie R. Kagan, PhD, Stephen J. Angello Professor of Electrical and Systems
INTERACTIONS IN SILICON - METAL NANOCAVITIIES FOR SILICON
PHOTONICS AND THERMOPLASMONICS
This work is licensed under the Creative Commons Attribution- NonCommercial-ShareAlike 3.0 License
To view a copy of this license, visit
I would like to take this opportunity to first thank my supervisor Dr. Ritesh
Agarwal, whose esteemed guidance and support has helped me tremendously in these
past five years. I would also like to thank my thesis committee members (past and
present) Dr. Nader Engheta, Dr. Cherie Kagan, Dr. Chris Murray and Dr. Ertugrul
Cubukcu for providing valuable counsel and insights. I would like to thank Dr. Carlos
Aspetti, former member of the Agarwal group for his guidance early on in my PhD; and
Jacob Berger and Rob Middleton for helping me navigate difficult times. The current and
former members of the Agarwal group have made these years truly transformative and
memorable; I would like to thank Dr. Joohee Park, Dr. Mingliang Ren, Dr. Pavan Nukala,
Wenjing Liu, Dr. Liaoxin Sun, Dr. Bumsu Lee, Dr. Sajal Dhara, Dr. Rahul Agarwal,
Stephanie Malek and Gerui Liu, for all their insightful scientific discussions.
I must not forget to mention other members of my PhD cohort- Dan, Frank and
Nick, and friends from Penn Taekwondo- Becky, Jessie, Tom, Robin and Kevin for
enriching my life these past five years.
Lastly, and most importantly, I want to thank my family especially my father who
always strived to bring happiness in my life, my mother for always standing beside me,
my sisters for make me believe in me, my brother in laws for supporting me in the most
ENGINEERING PHONON, PHOTON, ELECTRON AND PLASMON
INTERACTIONS IN SILICON - METAL NANOCAVITIIES FOR SILICON
PHOTONICS AND THERMOPLASMONICS
Ritesh Agarwal, PhD
Silicon photonics offers a cost effective solution to achieve ultrafast data
processing speeds. But due to its indirect bandgap structure, making lasers from silicon is
extremely difficult. Thus research has focused on nonlinear Raman processes in silicon as
a method to achieve optical gain. Silicon nanowires provide an interesting platform for
enhancing these nonlinearities because of their small size, geometry and relevant length
scales. In the current work Raman measurements done on silicon nanowires reveal that
up to twelvefold enhancement in Stokes scattering intensity and fourfold enhancement in
anti Stokes scattering intensity can be attained depending on cavity structure and size,
and excitation wavelength. In some cavities Stokes intensity depends on the sixth power
of pump intensity, indicating extreme nonlinearity. Numerical calculations, done to
understand the mechanism of these results indicate that silicon nanowires confine light to
highly intense electric field modes inside the cavity which lead to stimulated Stokes and
anti Stokes Raman scattering. Cavity modes can also be tuned to enhance the relative
emission of either one of anti Stokes or Stokes photons which could enhance cavity
cooling. These results would enable the development of smallest monolithically
intense electric field inside the nanowire could also be used to enhance the degree of
plasmon excitation in metallic nanoparticles. Silicon nanowires coated with a 10 nm thick
gold film lead to strong plasmon excitation in gold and high cavity absorption which
enable the cavity to heat up to temperatures of 1000K at relatively low pump powers. The
cavities also give the ability to measure temperature attained during plasmon excitation
and control the plasmon resonance wavelength. Because of the strong heating and
plasmonic effects, these cavities show enhanced evolution rates of hydrogen, a crucial
ACKNOWLEDGMENT ... IV
LIST OF TABLES ... IX
LIST OF FIGURES/ILLUSTRATIONS ... X
CHAPTER 1. INTRODUCTION ... 1
1.1 Case for nanoscale silicon photonics ... 1
1.2 Recent advances in silicon photonics ... 3
1.3 Raman scattering and Raman lasing ... 8
1.4 Relation between Raman scattering, phonon occupation number and temperature of the system ... 12
1.5 Localized surface plasmons and thermoplasmonics ... 15
1.6 Current work ... 19
CHAPTER 2: STIMULARED RAMAN SCATTERING IN SILICON NANOWIRES ... 27
2.1: SRS in nanostructures ... 27
2.2 Motivation ... 28
2.3: Cavity fabrication and experimental details ... 29
2.4: Optical Measurements on bulk silicon and bare silicon nanowires ... 34
2.5: Concluding remarks on SRS on bare silicon nanowire ... 50
2.6: SRS on silicon-gold cavities ... 52
2.7 Estimation of gain coefficient ... 59
2.8 Raman scattering in silicon-silver cavities and fano interactions... 61
2.9 A note on peaking narrowing during lasing ... 66
CHAPTER 3: CAVITY EFFECTS ON BOSE EINSTEIN DISTRIBUTION OF
PHONONS ... 78
3.1 Motivation ... 78
3.2 Bose Einstein Distribution and Temperature ... 79
3.3 Experimental details and measurements in bulk silicon ... 81
3.3 Anti Stokes – Stokes intensity ratios in silicon nanowire ... 84
3.4 Discussion ... 89
3.5 Measurements in silicon-gold cavities ... 91
3.6 Variance of anti Stokes/Stokes ratio on temperature ... 97
3.7 Concluding remarks and future work ... 106
CHAPTER 4: ENHANCED HEATING AND LOCALIZED SURFACE PLASMONIC ACTIVITY IN SILICON-GOLD NANOCAVITY ... 110
4.1 Motivation ... 110
4.2 Sample preparation and Experimental... 112
4.3 Optical measurements on a silicon wafer ... 116
4.4 Optical measurements on silicon nanowires ... 117
4.5 Thermal stability measurements on the cavity ... 132
4.6 Conclusions and future work ... 139
CHAPTER 5: CONCLUSIONS AND FUTURE WORK... 144
5.1: Conclusions ... 144
TABLES Page No.
Table 2.1: Total cavity losses at different wavelengths 51
Table 3.1: Anti Stokes to Stokes ratios in bulk silicon at different wavelengths. Experimental values are ratios of experimentally measured scattering intensities at anti Stokes and Stokes wavelength. FDTD calculations refer to the ratio of average electric field intensity inside the nanowire at the anti Stokes and Stokes wavelength.
Table 3.2: Anti Stokes to Stokes scattering intensity ratio for three silicon samples at room temperature using a 660 nm pump. The numbers adjacent to the nanowires are the diameters of the nanowire
Table 3.3: Comparison of calculations for ratio of average electric field intensity in the nanowire at anti Stokes and Stokes wavelength with the ratio of experimental scattering intensity at anti Stokes and Stokes wavelength for silicon nanowires of diameter 220 nm and 280 nm and for bulk silicon. The values have been normalized with the corresponding bulk values.
FIGURES/ ILLUSTRATIONS Page No.
Figure 1.113: Energy – momentum band diagram of a direct (InP) and an indirect (Si) bandgap semi conductor showing major charge carrier transition processes
Figure 1.220: Continuous wave Raman silicon laser: a) Schematic layout of silicon waveguide used in the Raman laser experiment; b) Silicon Raman laser output power as a function of the input pump power at a reverse bias of 25 and 5 V. Pump wavelength: 1,550 nm; laser wavelength: 1,686 nm. Error bars represent standard deviations
Figure 1.321: Layout of the silicon ring laser cavity with a p-i-n structure along the waveguide
Figure 1.428: Schematic diagram of (a) Stokes and (b) Anti Stokes, Raman scattering
Figure 1.5: Schematic showing Stimulated Raman Scattering 10
Figure 2.1: Schematic of Raman measurements on a bare nanowire 31
Figure 2.2: Schematic of Raman measurements on a metal coated nanowire 31
Figure 2.3: Scanning electron microscopy image of the cross section of a silicon nanowire coated with 360 nm gold
Figure 2.4: a) Power dependent Stokes Raman spectra of bulk Silicon using a 660 nm pump; b) Integrated Stokes intensity vs. pump power for bulk silicon. The dashed line represents the linear extrapolation of Stokes intensity from the lowest laser power
Figure 2.5: a) Fano coupling factor 1/q vs. laser power for bulk silicon with a 660 pump; b) Temperature (left vertical axis) and FWHM increase (right vertical axis) vs. pump power for bulk silicon.
Figure 2.6: Electric field intensity distribution in bulk silicon. a) Spatial distribution of electric field intensity inside the cavity at 660 nm; b) Average electric field intensity inside silicon as a function of wavelength. The thick
thin right vertical dashed line represents the position of Stokes wavelength.
Figure 2.7: Raman spectroscopy of bare silicon nanowire of diameter 100 nm with a 532 nm pump. a) Power dependent Raman spectra; b) Integrated Stokes Raman intensity as a function of laser power; c) Integrated Stokes Raman intensity vs. laser power in log-log scale; d) Asymmetry parameter 1/q vs. laser power
Figure 2.8: Electric field intensity distribution inside a bare silicon nanowire of diameter 100 nm. a) Average electric field intensity inside the silicon nanowire as a function of pump wavelength. Vertical dashed lines represent pump and Stokes wavelength from left to right; b, c) Spatial electric field intensity distribution inside the silicon nanowire at pump (532 nm) and at Stokes wavelength (547 nm) respectively. Circles represent silicon nanowire cross section. Inner core corresponds to the silicon nanowire and outer shell corresponds to the 2 nm thick silicon oxide layer. The horizontal straight line represents the substrate/air interface.
Figure 2.9: Effect of temperature on SRS in a bare silicon nanowire of diameter 100 nm at a 532 nm pump. a) Temperature (left vertical axis) and FWHM increase (right vertical axis) vs. pump power for the nanowire; b) Dependence of average electric field intensity inside the nanowire as a function of temperature. Inset shows the product of the electric field intensity at pump and at Stokes wavelength as a function of temperature; c) Experimentally measured temperature dependence of Stokes scattering intensity as a function of temperature for bulk silicon. The dotted line represents the scattering intensity predicted from the empirical model by Compaan et.al; d) Stokes scattering intensity for silicon nanowire shown in figure 2.7b corrected for temperature using the empirical relation by Compaan et.al
Figure 2.10: Electric field intensity inside a bare silicon nanowire of diameter 100 nm. a) Average electric field intensity inside the cavity as a function of pump wavelength. Vertical dash line represents the pump and the Stokes wavelength from left to right; b, c) Spatial electric field intensity distribution inside the cavity at pump (660 nm) and at Stokes wavelength (683 nm) respectively. The circles represent the silicon nanowire cross section. The inner core is the silicon nanowire and the outer shell is the oxide layer. The horizontal straight line is the substrate/air interface.
Figure 2.11: SRS in a nanowire without a cavity mode- bare silicon nanowire of diameter 100 nm excited with a 660 nm pump: a) Pump power dependence of integrated Stokes intensity; b) Temperature (left vertical axis) and FWHM increase (right vertical axis) vs. pump power for the nanowire; c) Temperature corrected Stokes scattering intensity for silicon nanowire shown in figure
Figure 2.12: SRS without a cavity mode- bare silicon nanowire of diameter 125 nm excited with a 532 nm pump. a.) Electric field intensity distribution inside a bare silicon nanowire of diameter 125 nm in TE polarization. a) Average electric field intensity inside the cavity as a function of pump wavelength. The vertical arrows represent the pump and the Stokes wavelength from left to right; b) Pump (532 nm) power dependence of integrated Stokes intensity
Figure 2.13: Electric field intensity distribution inside a bare silicon nanowire of diameter 225 nm. a) Average electric field intensity inside the cavity as a function of pump wavelength. Vertical dash line represents the pump and the Stokes wavelength from left to right; b, c) Spatial electric field intensity distribution inside the cavity at pump (660 nm) and at the Stokes wavelength (683 nm) respectively. The circles represent the silicon nanowire cross section. The inner core is the silicon nanowire and the outer shell is the oxide layer. The horizontal straight line is the substrate/air interface.
Figure 2.14: SRS in a bare nanowire of diameter 225 nm with a 660 nm pump: a) Pump power dependence of integrated Stokes intensity; b) a log-log plot of pump power dependence of Stokes intensity; c) Temperature (left vertical axis) and FWHM increase (right vertical axis) vs. pump power for the nanowire; d) Temperature corrected Stokes scattering intensity for silicon nanowire in figure 2.14a
Figure 2.15: Stimulated Raman Scattering in gold coated silicon nanowire of diameter 235 nm with a 660 nm pump: a) Power dependent Stokes Raman spectra of the silicon nanowire of diameter 250 nm; b) Integrated Stokes intensity as a function of laser power; c)Log-log plot of integrated Stokes intensity as a function of laser power, inset is the zoomed in version of the same graph showing the onset of SRS ; d) Fano interactions parameter 1/q as a function of laser power
Figure 2.16: Mechanism of Stimulated Raman Scattering- gold coated silicon nanowire of diameter 235 nm with a 660 nm pump: a) Average electric field inside the cavity as a function of excitation wavelength. Vertical dash line represents the pump and the Stokes wavelength from left to right; b,c) electric field intensity distribution inside the silicon nanowire cavity at the pump wavelength (660 nm) and the Stoke’s wavelength (683 nm). Black circles represent the nanowire. Horizontal line is the substrate-gold interface
Figure 2.17: Effect of Temperature on Stimulated Raman Scattering- gold coated silicon nanowire of diameter 235 nm with a 660 nm pump: a): Temperature (left vertical axis) and increase in FWHM (right axis) of the cavity as a function of pump power. Inset shows the product of the electric
b) FDTD calculation of field confinement in the cavity as a function of temperature; c) Temperature corrected experimental integrated Stokes intensity as a function of laser power of silicon nanowire; d) Log-log plot of temperature corrected Stokes intensity vs. pump power
Figure 2.18: Wavelength and size distribution of average electric field intensity inside the silicon nanowire in TM polarization. a.) in bare silicon nanowire; b) in gold coated silicon nanowires. Green and red vertical dashed lines represent the position of the available pump wavelengths using which SRS experiments were conducted.
Figure 2.19: Electric field confinement in silver coated silicon nanowires: a) Wavelength and size distribution of average electric field intensity inside the silicon nanowire in TM polarization; b) Diameter dependence of average electric field intensity at the pump and at the Stokes wavelength.
Figure 2.20: Raman scattering in silver coated silicon nanowire: a, b) Power dependent anti Stokes and Stokes Raman spectra; c) Fano interaction parameter as a function of laser power; d) Temperature (left vertical axis) and increase in FWHM (right vertical axis)as a function of laser power
Figure 2.21: Stimulated Raman scattering in silver coated silicon nanowire: a) Integrated Stokes intensity as a function of pump power for the nanowire in figure 2.20; b) Log-log plot of integrated Stokes intensity vs. pump power for the same nanowire.
Figure 2.22: Fano asymmetry parameter 1/q vs. laser power for a silver coated silicon nanowire showing saturation in 1/q
Figure 2.23: Dependence of anti Stokes intensity on temperature: a.) Stokes intensity vs. temperature with a 532 nm pump24; b) Anti Stokes/Stokes ratio vs. temperature23; c)Anti Stokes intensity as a function of temperature.
Figure 2.24: Stimulated anti Stokes Raman scattering in gold coated silicon nanowire of diameter 230 nm using a 660 nm pump: a) Power dependence of integrated anti Stokes intensity; b) Temperature (left vertical axis) and increase in FWHM (right vertical axis)as a function of laser power; c) Temperature corrected integrated anti Stokes intensity vs. pump power; d) Dependence of average electric field intensity inside the silicon nanowire of diameter 230 nm on wavelength. Vertical dash line represents the anti Stokes and the pump and wavelength from left to right
Figure 3.1: Anti Stokes and Stokes Raman spectra of 3 silicon samples: bulk, nanowires of diameter 220 nm and 280 nm collected using a 660 nm pump. The three spectra have been normalized with the maximum of Stokes
Figure 3.2: Spatial electric field intensity profile inside the nanowires at: a, b) anti Stokes and Stokes wavelength for the silicon nanowire of diameter 220 nm; c, d) anti Stokes and Stokes wavelength for the silicon nanowire of diameter 280 nm.
Figure 3.3: Average electric field intensity inside the silicon as a function of wavelength for bulk silicon and two nanowires of diameters 220 nm and 280 nm.
Figure 3.4: Average electric field intensity at anti Stokes (638 nm) and Stokes (683 nm) wavelength inside the silicon nanowire as a function of nanowire diameter.
Figure 3.5: Comparison of experimental ratios (left vertical axis) and theoretical ratios (right vertical axis) (as defined in section 3.2). Left vertical axis: Dependence of anti Stokes to Stokes scattering ratio (relative to bulk) on nanowire diameter; Right vertical axis: Dependence of ratio of average electric field confinement at anti Stokes to Stokes wavelength (relative to bulk) on nanowire diameter.
Figure 3.6: Comparison of experimental ratios (left vertical axis) and theoretical ratios (right vertical axis) (as defined in section 3.2 in gold coated silicon nanowires at a) 660 nm; b) and at 532 nm.
Figure 3.7: Comparison of experimental ratios (left vertical axis) and theoretical ratios (right vertical axis) (as defined in section 3.2 in gold coated silicon nanowires in TE polarization at 660 nm;
Figure 3.8: Comparison of scattering intensity ratios (relative to bulk) in the same nanowire with different mode confinement at Stokes and anti Stokes wavelength.
Figure 3.9: Comparison of a) anti Stokes to Stokes scattering intensity ratio (AS/St intensity); and b) phonon population ratio; at elevated temperature for a nanowire with bulk like anti Stokes to Stokes scattering intensity ratio
Figure 3.10: Comparison of a) anti Stokes to Stokes scattering intensity ratio (AS/St intensity); and b) phonon population ratio; at elevated temperature in a bare silicon nanowire of diameter 330 nm
Figure 3.11: Comparison of a) anti Stokes to Stokes scattering intensity ratio (AS/St intensity); and b) phonon population ratio; at elevated temperature, in a silicon nanowire of diameter 60 nm, coated with a thick gold shell
(AS/St intensity); and b) phonon population ratio; at elevated temperature, in a silicon nanowire of diameter 234 nm; c-d) similar comparison for a silicon nanowire of diameter 190 nm coated with a thick gold shell
Figure 3.13: “Population”-inversion: Anti Stokes to Stokes scattering intensity ratio (AS/St intensity) showing greater intensity of anti Stokes scattering than Stokes scattering
Figure 4.1: Scanning electron microscopy (SEM) image of a gold coated silicon nanowire (scale bar: 200 nm)
Figure 4.2: Schematic of cavity. Green and red arrows indicate direction of K vector of incident wave and back scattered Raman wave respectively, solid and dashed black arrows indicate direction of polarization of electric field of incident light in transverse magnetic (TM) and transverse electric polarization (TE) respectively.
Figure 4.3: Schematic of cavity for photocatalysis experiments 115
Figure 4.4: a-b) Power dependent Raman spectra using a 532 nm pump of a) Bare silicon wafer; b) Silicon wafer coated with 10 nm gold. Legend indicates pump power in mW.
Figure 4.5: Raman spectra of a bare silicon nanowire (100 nm diameter) at different incident powers using 532 nm wavelength in the TM polarization.
Figure 4.6: Extra ordinary heating of gold coated silicon nanowires: a) Temperature vs. laser power for the gold coated nanowire calculated from the Raman spectra shown in figure 4.5) and also for the same nanowire after coating 10 nm gold; b) Computational simulations of absorption spectra of the nanowire cavity for gold coated and bare nanowire of diameter 100 nm in TM and TE polarization. Vertical green and red arrows indicate the wavelength of the pump (532 nm and 660 nm)
Figure 4.7: Mechanism of heating: a-b) Electric field distribution inside the cavity in TM polarization for bare and 10 nm gold coated nanowire of diameter 100 nm respectively at 532 nm
Figure 4.8: Heating in a cavity with off resonance excitation: a) Temperature vs. laser power for gold coated and bare nanowire of diameter 100 nm in TM polarization at 660 nm excitation; d) Electric field distribution inside the silicon nanowire of diameter 100 nm coated with 10 nm gold in TM polarization at 660 nm
laser power of a silicon nanowire of diameter 100 nm coated with 150 nm gold in TM polarization (532 nm excitation), inset shows the schematic of the experiment; b) Computational simulations of absorption spectra of the metal-nanowire cavity in a)
Figure 4.10:Heating in Ti coated cavities: a) Computational simulation of the absorption spectra of silicon nanowire of diameter 100 nm coated with 10 nm Ti; b) Experimentally observed temperature vs. laser power of the cavity in (a) at 532 nm.
Figure 4.11: Higher absorption in cavity modes: a-d) Computational simulations showing diameter and wavelength dependence of absorption modes in TM polarization for a bare silicon nanowire, hollow gold shell, bare silicon nanowire + hollow gold shell, and for cavity respectively, color bar represents % of absorbed incident power
Figure 4.12:Cavity size tuning of resonant mode: a) Computational simulations of absorption spectra of gold coated and bare nanowire of diameter 240 nm in TM and TE polarizations (660 nm excitation); b) Temperature vs. laser power of cavity in a)
Figure 4.13:Wavelength and size dependence of resonant modes:a,b)
Computational simulations showing diameter and wavelength dependence of absorption modes in TM and TE polarization respectively, color bar
represents % of absorbed incident power
Figure 4.14: a) Hydrogen evolution from the silicon-gold-titania nanocavities
gold-titania catalyst and from silicon-gold; b) Schematic of
silicon/gold/titania cavity catalyst
Figure 4.15: Cavity stability tests: Temperature – a) and Raman intensity – b) vs. laser power for three repeated cycle at the same spot on the nanowire with a maximum temperature of 630 K. c, d) SEM images of the nanowire on which the test was carried out and of the film on which same cycle of laser irradiation was repeated. Scale bar is 500 nm in each image.
Figure 4.16: Cavity stability tests: Temperature – a) and Raman intensity – b) vs. laser power for three repeated cycle at the same spot on the nanowire with a maximum temperature of 750 K; c, d) Similar data except with a maximum temperature of 950 K
Figure 4.17: SEM image of the nanowire region kept at 950 K. Scale bar is 500 nm
vs. laser power for three repeated cycle at the same spot on the nanowire with a maximum temperature > 1000 K
Figure 4.19: SEM image of the nanowire region heated to a temperature > 1000 K. Scale bar is 200 nm
CHAPTER 1. Introduction
1.1 Case for nanoscale silicon photonics
The advances in the CMOS technology have greatly enhanced processor speed of
devices. However, device size is expected to reach saturation soon1 with Intel already
working on a 14 nm transistor2. Moreover, with the ever increasing demand for faster
speeds and larger bandwidths from interconnects, copper interconnects are expected to
soon lag behind the requirements3. Both of these would greatly affect the potential speeds
at which chips could operate. Optical interconnects provide an alternative, allowing much
faster speeds and larger bandwidths and are already being used to connect racks of
equipment that span 1-100 meters. Over the next decade they are expected to slowly
make way into backplane communication- connecting separate printed circuit boards over
a distance of 20-100 cm, and eventually to chip to chip applications, spanning less than
20 cm 3. These would allow for much faster device speeds and faster communication
between different components of a chip. They would also directly greatly increase the
rate at which data can be transferred across a network.
Silicon because of its low cost and compatibility with the CMOS industry offers
itself as the obvious choice for optical interconnect material. Using silicon would allow
for easy assembly and integration of optical components within the existing devices
leading to much lower cost given that packaging and assembly account for ~ 60-70% of
explored. Decade long research has opened up exciting possibilities; with silicon laser5
and optical modulation being realized6, which could dramatically revolutionize the
industry. To give some perspective, copper interconnects typically allow for a speed of
~100Mbits/sec and the best ones available can potentially go as fast as
10-20Gbits/second3. Today silicon devices can modulate signals electro-optically and
process data at speeds higher than that7.It can be used to process optical signals at speeds
of 100Gbit/s and beyond78. Tbits/s speed is the next goal9 and while the developments so
far have been promising, there are still a variety of issues that need to be addressed.
Silicon based photonic devices typically have large footprints (>10 μm). Hence they
require higher operating powers; which along with their size-mismatch with electronic
components limits their potential for ultra dense device integration. High manufacturing
cost for high volume production, high heat generation originating from high power
requirements further limit the applications. Moreover some silicon-germanium (or III-V)
hybrid components are still required especially for applications as a lasing source, which
further complicates the integration steps. Therefore, new advances in materials design,
fundamental understanding of nanoscale optical physics and innovative optical
engineering are required to solve this problem.
Nanoscale silicon photonics could go a long way in addressing these issues.
Efficient silicon photonics at the nanoscale would bring down the size of optical
components making integration much easier. Nanowire geometry as well as all (only)
nanoscale components would also work at much lower operating power and voltages
(possibly a few orders of magnitude lower). Given that interconnects today consume
about 80% of the microprocessors power; this would bring about a dramatic decrease in
the power consumption10. Lower powers consumption would decrease the amount of heat
that needs to be removed from the system bringing the load on the cooling
infrastructure10. Given the amount of heat that can be removed from a chip in cost
effective manner is expected to be constant in the foreseeable future10, minimizing power
losses is extremely important for larger scale integration of devices. An all silicon laser at
the nanoscale which could be easily integrated would be another big step which would
greatly reduce the power requirements both in terms in operating power and cooling
infrastructure, making the system more energy efficient and economical, as well as make
device integration feasible allowing for much faster speeds especially required in data
centers and super computers.
Other potential applications areas for silicon photonics include
telecommunications, optical sensing, biomedical applications, imaging, quantum
cryptography and atmospheric sensing and monitoring1112.
1.2 Recent advances in silicon photonics
Silicon is an indirect band gap material with a bandgap of 1.12 eV4. Conventional
lasers employ direct band gap semiconductors in which the maxima of the valence band
hole recombination event almost always results in a photon emission (figure 1.1 )
leading to high quantum efficiency. However for silicon, the minima of conduction band
and the maxima of valence band do not lie at the same point in k-space (Figure 1.113). As
a result non radiative processes such as Auger recombination and free Carrier absorption
(FCA) dominate carrier relaxation processes. The rate of radiative recombination is about
6 orders of magnitude lower than the rate of non-radiative recombination13. Thus it is
extremely difficult to make silicon lasers via the conventional electron-hole
One of the alternate ways that has been exploited to make a silicon laser is by
using Stimulated Raman scattering (SRS, discussed in next section). But high losses from
Figure 1.113: Energy – momentum band diagram of a direct (InP) and an indirect (Si)
difficult to achieve net cavity gain14 15. Liu et.al showed via simulations that the free
carrier density via two photon absorption (TPA) in a silicon waveguide can be
significantly reduced if the pump width is small compared to the carrier lifetime; which
led to the observation of SRS, a precursor for Raman lasing, being observed in bulk
silicon for the first time using pulsed laser pumping16. The first silicon Raman laser was
also built using pulsed lasing17 with a lasing threshold of 9 watts.
The mechanisms used with pulsed lasing could not be used with a continuous
wave pumping and the free carrier density with continuous pumping is always high. But
losses could still be reduced by reducing the effective carrier lifetime18. To decrease the
carrier transit time Jones et.al19 used a p-i-n junction which was formed by depositing a
p+ layer and an n- layer on either side of the waveguide. The carrier transit time (free
carrier lifetime) could be varied by applying different reverse bias voltage across this
junction. Higher the reverse bias voltage lowered the carrier transit time leading to lower
losses. Lowest carrier life time of ~ 1 ns, with a reverse bias voltage of 25V, was
reported. Using this they were able to show, net optical gain with continuous wave
pumping. This was followed by lasing using continuous wave pumping with the
application of a reverse bias in a ‘S’ shaped cavity of size 4.8 cm (figure 1.2a)20. In this
cavity, lasing threshold and conversion efficiency (of pump to Stokes wavelength) was a
direct function of losses in the cavity. Lower losses decreased the lasing threshold and
increased conversion efficiency while higher losses increased the lasing threshold and
output characteristics in figure 1.2b). Note that this threshold power values correspond to
the amount of power coupled into the cavity and not the total pump power. Figure 1.2 20
shows the schematic of this cavity and the output of laser for two reverse bias voltages.
The first monolithically integrated laser (schematic in figure 1.321) was made by
forming a racetrack resonator cavity with a length of 3 cm and the bent radius was 400
µm. The quality factor of the cavity was calculated to be ~ 6E5, anddepending on the
device architecture and applied reverse bias voltage, lasing threshold powers in between
~150 and 250 mW were reported21. This laser could be integrated on the chip and paved
way for a plethora of applications. More recently, a cascaded laser22 and a 0-reverse bias
voltage laser23 have also been made, primarily by decreasing cavity losses and increasing
the cavity quality factor.
Figure 1.220: Continuous wave Raman silicon laser: a) Schematic layout of silicon
waveguide used in the Raman laser experiment; b) Silicon Raman laser output power as a function of the input pump power at a reverse bias of 25 and 5 V. Pump
While the developments in achieving optical amplification have been
phenomenal, these devices have the footprint of a few centimeters which increases the
power consumption and also makes it difficult to integrate these lasers with other
nanoscale components of the chip. Such larger cavities are required because although the
Raman gain for silicon is higher than Raman gain for a lot of other materials, the gain
value is still very small due to low Raman scattering cross section. These lasers also
require cavities with very high quality factors as well as application of a reverse bias
voltage to further decrease cavity losses.
Hybrid silicon lasers have also been fabricated which have a III-V semiconductor
gain medium integrated with a SOI waveguide24252627. These hybrid lasers have a
device footprint of a few microns and require a few 100 of µA of current for lasing but
are harder to fabricate on-chip, involving multiple complicated fabrication steps which
1.3 Raman scattering and Raman lasing
Raman Scattering is the process by which photons get inelastically scattered
from phonons (lattice vibration modes) in a lattice, leading to new photons, shifted
(Raman shift) in energy from the incident photons by an amount equal to the vibrational
energy of the phonons. The up-converted photons are anti-Stokes scattered while the
down shifted photons are Stokes scattered. The relations in between photon frequencies
for Stokes and anti Stokes scattering can be summarized by the following two
At room temperature Stokes scattering and hence Stokes photons are more
common than anti-Stokes scattering and anti-Stokes photons. This is because at room
temperature, a larger fraction of phonons are in the ground state. Figure 1.428 shows the
First order and higher order Raman scattering processes:
Spontaneous Raman scattering is a first order optical process in which Stokes
intensity is proportional to the first power of incident laser (pump) intensity. This is
typically observed at low pump powers.
Stimulated Raman scattering (SRS) is a third order optical process in which
Stokes intensity is proportional to the second power of the pump intensity and first power
of probe (at Stokes wavelength) intensity. Accordingly a probe wavelength (λSt), in a
Raman active (gain) medium, is amplified in the presence of a pump wavelength (λP) if
the energy difference in between the two wavelengths is equal to the Raman shift of the
material of the medium. This is explained in the schematic in figure 1.5. The probe beam
while propagating in the medium, experiences attenuation and as a result the intensity of
beam coming out of the medium is less than the intensity of light going into the medium.
In the presence of a pump beam, the intensity of the probe beam coming out of the
pump beam if the difference in the energy of pump and probe photons is equal to the
Raman shift of the medium. This apparent increase in intensity is because of SRS. If the
losses in the system are minimized enough and the length of the medium is long enough,
then the intensity of the probe beam coming out of the cavity could be greater than the
intensity going in, leading to a net gain. This happens when the gain from SRS is greater
than the cavity losses. To convert this gain from SRS into a laser, mirrors can be placed
on either side of the cavity to keep the probe beam into the medium leading so that it can
experience gain leading to build up of intensity of the probe beam resulting in lasing
(assuming net roundtrip gain is positive).
I = Intensity of laser
Typically in operation of a Raman laser, only a pump beam is used. Stokes
scattered wave acts as the probe beam and is amplified as a result of Raman gain. Thus
during SRS, Stokes intensity is super linearly dependent on the pump power experiencing
gain as it propagates in the medium. The proportion of increase in Stokes emissions is
is positive, a laser can be built. Raman scattering cross section for materials are extremely
small and typically only one photon in a few million is Raman scattered. As a result the
gain coefficient associated with Raman scattering is also very small. For silicon it is of
the order of 10 GW/cm19 which although is much larger than the corresponding value for
silica fibers but is inherently much smaller. Just increasing the propagation distance in the
gain medium is not enough to achieve Raman gain/lasing. Minimization of cavity losses
is also very critical as was discussed in the last section. As a result Raman lasers
typically require long propagation lengths for the gain to build up in the cavity. It is for
this reason that SRS reports in nanostructures have been few.
Stimulated anti Stokes Raman Scattering (SARS) refers to the process in
which the anti Stokes scattering intensity experiences a gain in the Raman medium. The
anti-Stokes intensity is proportional to the second power of pump intensity and the first
power of anti Stokes intensity. Conceptually it is exactly similar to SRS29 except is
observed less commonly due to much lower anti Stokes scattering cross section. One of
the reasons for that is the fact that at room temperature only a small fraction of phonons
are present in the higher energy levels from where they could transition to ground state to
emit an anti Stokes scattered phonon. Nevertheless anti Stokes lasing has been
demonstrated in BaWO4 crystal by placing the crystal at an angle to the incident beam so
that there is non-collinear phase matching for the generation of first anti Stokes wave
1.4 Relation between Raman scattering, phonon occupation number and
temperature of the system
Temperature Determination from Bose Einstein distribution
Since phonons are bosons they follow the Bose Einstein distribution.
Accordingly, the probability that a particle will have energy E is given by the expression:
1 1 )
E K T
where A is a constant (1 for phonons), T is the temperature and KB is the Boltzmann
constant. Since the anti Stokes and Stokes line correspond to the absorption and emission
of an optical phonon, the ratio of their intensities IAS and ISt is given by31:
1 o o St AS N N I I (1.3b)
where No is the equilibrium occupation number of the q = 0 optical phonon of frequency
ωo is given by34
) 1 ) (exp( T K N B o o
where ħ is the Planck’s constant. This simplifies equation 1.3b to34:
) exp( T K I I B o St
the ratio of anti Stokes scattering to Stokes scattering. Various relations similar to
equation 1.3d have been suggested. And while there is agreement on the general form of
this expression various proportionality constants have been proposed to replace the ‘1’
before the exponential term3233 343536. Most of these expressions have been widely used
by various researchers for temperature determination applications. The general form of
this expression is presented in equation 1.4.
T K I
Temperature determination from change in Raman shift
Temperature of the system can also be determined by the temperature dependent
phonon energy (Raman shift) or uncertainty in phonon energy which is determined by the
full width half maximum (FWHM) of the Raman peak. Lattice anharmonicity typically
leads to a decrease in the phonon energy and an increase in the uncertainty of the phonon
energy which leads to a red shift and a broadening of the Raman peak37 38. For silicon,
the temperature dependence of this red shift and change in FWHM is well understood and
various theoretical models have been developed and verified experimentally for the same.
The model developed by Balkanski et.al39 (equations 1.5 and 1.6), has been widely used
for temperature calculations from change in Raman shift for bulk silicon as well as
model has been used to determine temperature in the current work presented in chapters
2, 3 and 4.
) ) 1 ( 3 1 3 1 ( ) 1 2 1 ( * ) ( 2
x y y
where ∆ is the change in Raman shift, T is the temperature, C and D are constants
and were determined to be -2.96 -0.174 by Balkanski et.al.
T k x B o 2 and T k y B o 3
Other models relating phonon energy to temperature (for silicon) have also been
proposed. One of them predicts the change in Raman shift to be .022 cm-1 for every 1K
rise in temperature4445.
Phonons and Temperature
Temperature of a system is a measure of energy of the system. In crystalline
solids, most of that energy is stored in the form of lattice vibrations. A system at a higher
temperature will have more vibrational energy and the occupation number for phonons
will be higher. A system at a lower temperature would have lower vibrational energy and
most of the phonons will be in ground state (lower occupancy number). It follows that in
order to decrease the temperature of a system, one only needs to bring phonons from
to the ground state (phonon annihilation), it leads to cooling of the system. Stokes
scattering, on the other hand leads to generation of a phonon which would lead to
heating. Cavity heating is a major concern for operation of Raman lasers46 and much
work has focused on decreasing the heating by increasing the anti Stokes scattering in the
cavity47 48. If somehow the anti Stokes scattering could be enhanced in the system, the
material would lose heat more quickly. But since Stokes scattering is always greater than
anti Stokes scattering (because of low occupancy number) more phonons are always
being generated than are being annihilated. If somehow the relative intensity of anti
Stokes scattering were to be increased, it could bring about optical cooling in materials,
even in indirect bandgap semi-conductors.
1.5 Localized surface plasmons and thermoplasmonics
Metal nanoparticles possess interesting optical properties because of presence of
collective oscillations of electrons called plasmons. These plasmons lead to generation of
high electric fields close to the metal surface, the extent of enhancement of field
depending on the material, its structure and the surrounding medium. The hot electrons
generated via plasmon excitation can either be used to aid electron transfer in chemical
reactions49 or to generate local heat for various applications such as photothermal therapy
for cancer treatment, nano-surgery, photothermal drug delivery, photothermal imaging
and nanochemistry50. There has been a growing interest in exploring various metallic
Gold is the most commonly used plasmonic metal because of its inert nature and
its plasmonic resonance lying in the visible to infrared range51 52. The success of a
metallic nanostructure for plasmonic applications depends on the ease with which the
structure can be synthesized, the lifetime of the structure and the control it offers over
tuning its properties. A variety of plasmonic structures such as nanospheres and
nanorods53, dielectric core-metallic shells54, nanomatryushkas (metal-dielectric-metal
core-shell-shell structure)55 and metallic ring/disc cavities56 have been engineered for
Of all of these structures, nanospheres are the easiest to synthesize. Irradiation of
the light on the nanosphere at the plasmon resonance leads to high absorption and
scattering efficiencies because of which they find uses as localized heat generators. The
plasmon resonance depends on the diameter of the nanosphere and a larger diameter
typically leads to red shifting of the plasmon resonance due to retardation effects53. But
because of this nanospheres only allow a narrow spectrum in which the plasmon
resonance wavelength could be tuned. This makes them unsuitable for a variety of
nanoscale applications. It is difficult to tune the resonance wavelength to infrared regions
for therapeutic applications. This problem is overcome by use of geometrically
asymmetric shapes such as rods. The asymmetric shape leads to red shifting of the
plasmon resonance due to retardation effects and provides a broader resonance spectrum.
Resonance wavelength is typically found to change with the aspect ratio of the rods53.
resonance in the infrared regions for particles of small size54. Nanomatryushkas which
are core-shell-shell structures of metal-dielectric-metal provide better resonance
wavelength control at much smaller sizes compared to nanoshells because of additional
hybridized energy states arising out of interactions in between the inner and outer metal
structure. They also give the flexibility to control relative scattering and absorption cross
sections by changing the diameter of inner and outer metallic structures. Having a large
absorption cross section leads to generation of localized heat and applications in
Plasmonic structures have found use in a variety of biological in-vivo
applications. Cognet et.al used 10 nm gold particles for protein detection in cells based on
photothermal interference contrast57. Orozco used the heat generated from gold
nanomatryushkas and gold nanoshells for treating triple negative breast cancer tumors in
mice58. In plasmonic photothermal delivery, a therapeutic agent attached to a gold
nanoparticle, which acts as the carrier, is released at the target upon laser induced heating
of the nanoparticle59. Plasmonic nanostructures also have been used for various high
temperature applications. High temperatures have been attained in plasmonic structures
using laser irradiation and have been shown to promote nanowire growth60 61. A variety
of chemical reactions have shown enhanced reaction rates either due to high temperatures
which increase the speed of redox reactions . Generation of super heated water
vapor/steam using focused sunlight and gold nanoparticles was also shown 656667.
The ability to measure the change in temperature of the system as a result of
heating induced by the plasmonic system is critical since many applications require a
precise temperature control. Techniques to measure heat released or temperature change
exploit change in phase68, photoluminescence intensity69, fluorescence polarization
anisotropy70, Raman scattering71 or extended x-ray absorption fine structure72. In high
temperature systems temperatures measurements have been limited to estimates being
made using various chemical reactions62, 63, 64 or Stokes/anti-Stokes ratio66 or thermal
models60, 73 and only a few methods exits which work for temperatures beyond 100°C74
. In one the works Raman peak width of ZnO was used to measure temperature76 but it
has been shown that non-uniform heating which is likely to happen with localized heating
in nanostructures, causes additional peak broadening77 and hence may lead to an
overestimation of the temperature. Fano interactions as a result of scattering of
photogenerated charge carriers with phonons which is commonly observed in semi
conductors may also lead to broadening of Raman peak leading78 to additional errors in
temperature determination from peak width of Raman spectrum.
Limitations in existing plasmonic structures
Majority of the work on engineering plasmonic structures has focused on tuning
the plasmon resonance wavelength and little work has been done on increasing the
promoting interparticle interactions79. Thus the structures engineered thus far have either
been completely made out of a metal or have an inactive core such as silica. While such
core-shell structures lead to new hybridized energy states and have various advantages,
such systems limit the interactions between the metal and electric field of the light
because of the low refractive index of the core. Use of complex structures at high
temperatures is undesirable since gold is known to anneal at high temperatures80 which
could not only change the plasmon resonance drastically but also destroy the complete
structure itself. Thus a new strategy for plasmonic enhancement and wavelength control
could be great significance. Using a high refractive material such silicon for the core in a
core shell structure could have multiple advantages. The high refractive index core could
confine light to extremely small energy densities which could increase the degree of
plasmonic excitations. An active core could also provide temperature measuring
capability which could be extremely important in the field of catalysis.
Chapter 4 discusses the work done on silicon-gold cavities that have been
fabricated to enhance the plasmonic interactions in gold and the temperature measuring
capabilities of these cavities.
1.6 Current work
In the current work, interactions in between phonons, photons, electrons and
plasmons have been engineered by changing the structure and size of silicon nanowire
scattering. Alignment of the cavity mode with either of Stokes or anti Stokes wavelength
and the pump wavelength leads to strong confinement of electric field intensity inside the
nanowire which decreases the threshold for Raman non linear effects. A metallic layer on
of silicon helps the cavity dissipate heat faster. Fano interactions can also be tuned by
choosing an adequate metallic layer. Chapter 3 discuss the effects of selectively tuning
the cavity mode with either one of Stokes or anti Stokes wavelength on the anti Stokes to
Stokes scattering ratio.
In chapter 4 the discussion moves away from non linear optics onto plasmonics.
The chapter investigates how the intense electric field inside the silicon nanowire at
cavity mode resonance can be used to excite strong localized surface plasmons in thin
plasmonic metallic films covering the nanowire and its effect on the cavity temperature.
Nawrocki, W. Physical limits for scaling of integrated circuits. J. Phys. Conf. Ser.248, 012059 (2010).
Alduino, A. & Paniccia, M. Interconnects: Wiring electronics with light. Nat. Photonics 1, 153–155 (2007).
Sze, S.M. & Kwok K.N. Physics of semi conductor devices, third edition. (2006).
Fang, Z., Chen, Q. Y. & Zhao, C. Z. A review of recent progress in lasers on silicon.
Opt. Laser Technol.46, 103–110 (2013).
Leuthold J., Koos C., Freude W. Nonlinear silicon photonics. Nature Photonics 4, 535-544 (2010).
Paniccoa, M. Integrating Silicon photonics. Nat. Photonics4, 498–499 (2010).
Miller, D. A. B. Device requirements for optical interconnects to silicon chips. Proc. IEEE97, 1166–1185 (2009).
Rong, H. et al. Monolithic integrated Raman silicon laser. Opt. Express14, 6705–6712 (2006).
Paniccia, M. Integrating Silicon photonics. Nature Photonics 4, 498-499 (2010).
Liang D. & Bowers J.E. Recent progress in lasers on silicon. Nature Photonics 4; 511-517 (2010).
Rong, H., Liu, A., Nicolaescu, R. & Paniccia, M. J. Raman gain and nonlinear optical absorption measurements in a low-loss silicon waveguide. Appl. Phys. Lett.85, 2196– 2198 (2004).
Liang, T. K. & Tsang, H. K. Role of free carriers from two-photon absorption in Raman amplification in silicon-on-insulator waveguides. Appl. Phys. Lett.84, 2745–2747 (2004).
Liu, A., Rong, H., Paniccia M. et.al Net optical gain in a low loss silicon-on-insulator waveguide by stimulated Raman scattering. Optics Express 12 (18), 4261-4268 (2004).
Boyraz, O. & Jalali, B. Demonstration of a silicon Raman laser. Optics Express 12 (21), 5269-5273 (2004).
Liang, T. K. & Tsang, H. K. Efficient Raman amplification in silicon-on-insulator waveguides. Appl. Phys. Lett.85, 3343–3345 (2004).
Jones, R., Rong, H., Liu, A. et.al. Net continuous wave optical gain in a low loss silicon-on-insulator waveguide by stimulated Raman scattering. Optics Express 13 (2), 519-525 (2005).
Rong, H., Jones, R., Liu, A. et.al. A continuous-wave Raman silicon laser. Nature 433, 725-728 (2005).
Rong, H., Kuo, Y., Xu, S. et.al. Monolithic integrated Raman silicon laser. Optics express 14 (15), 6705-6712 (2006).
Rong, H., Xu, S., Kuo, Y. et.al. Low-threshold continuous-wave Raman silicon laser. Nature Photonics 1, 232-237 (2007).
Spuesens, T. et al. Improved design of an InP-based microdisk laser heterogeneously integrated with SOI. IEEE Int. Conf. Gr. IV Photonics GFP 202–204 (2009).
Fang, A. W. et al. Electrically pumped hybrid AlGaInAs-silicon evanescent laser. Opt.
Express14, 9203–9210 (2006).
Liang, D. et al. Electrically-pumped compact hybrid silicon microring lasers for optical interconnects. Opt. Express17, 20355–20364 (2009).
Van Campenhout, J. et al. A Compact SOI-Integrated Multiwavelength Laser Source Based on Cascaded InP Microdisks. IEEE Photonics Technol. Lett.20, 1345–1347 (2008).
Boyd, R.W. Nonlinear optics. Third edition (2008).
Wang, C. et al. Extracavity pumped BaWO4 anti-Stokes Raman laser. Opt. Express21,
Hart, T., Aggarwal, R. & Lax, B. Temperature Dependence of Raman Scattering in Silicon. Phys. Rev. B1, 638–642 (1970).
Tsu, R. & Hernandez, J. G. Temperature dependence of silicon Raman lines. Appl.
Phys. Lett.41, 1016–1018 (1982).
Fujimori, H., Kakihana, M., Ioku, K., Goto, S. & Yoshimura, M. Advantage of anti-Stokes Raman scattering for high-temperature measurements. Appl. Phys. Lett. 79, 937– 939 (2001).
Jellison, G. E., Lowndes, D. H. & Wood, R. F. Importance of temperature-dependent optical properties for Raman-temperature measurements for silicon. Phys. Rev. B28, 3272–3276 (1983).
Gupta, R., Xiong, Q., Adu, C. K., Kim, U. J. & Eklund, P. C. Laser-induced fano resonance scattering in silicon nanowires. Nano Lett.3, 627–631 (2003).
Doerk, G. S., Carraro, C. & Maboudian, R. Temperature dependence of Raman spectra for individual silicon nanowires. Phys. Rev. B80, 073306 (2009).
Haro, E., Balkanski, M. Wallis, R.F. & Wanser K.H. Theory of the anharmonic damping and shift of the Raman mode in silicon. Physical Review B 34(8), 5358-5367 (1986).
M. Balkanski, R. F. Wallis, ' and E. Haro . Anharmonic effects in light scattering due to optical phonons in silicon. Physical Review B 28 (4), 1928- 1934 (1983).
Konstantinović, M. et al. Raman scattering in cluster-deposited nanogranular silicon films. Phys. Rev. B66, 161311–1–4 (2002).
Niu, J., Sha, J. & Yang, D. Temperature dependence of the first-order Raman scattering in silicon nanowires. Scr. Mater.55, 183–186 (2006).
Piscanec, S. et al. Raman spectroscopy of silicon nanowires. Phys. Rev. B68, 2–5 (2003).
Adu, K. W., Gutiérrez, H. R., Kim, U. J. & Eklund, P. C. Inhomogeneous laser heating and phonon confinement in silicon nanowires: A micro-Raman scattering study. Phys.
Rev. B - Condens. Matter Mater. Phys.73, 1–9 (2006).
Doerk, G. S., Carraro, C. & Maboudian, R. Temperature dependence of Raman spectra for individual silicon nanowires. Phys. Rev. B80, 073306 (2009).
Khachadorian, S., Scheel, H., Colli, A., Vierck, A. & Thomsen, C. Temperature dependence of first- and second-order Raman scattering in silicon nanowires. Phys.
Status Solidi247, 3084–3088 (2010).
Koechner, W. Solid-state laser engineering. Fourth Edition (1996).
Vermeulen, N., Debaes, C., Muys, P. & Thienpont, H. Mitigating Heat Dissipation in Raman Lasers Using Coherent Anti-Stokes Raman Scattering. Phys. Rev. Lett.99, 093903 (2007).
Vermeulen, N., Debaes, C. & Thienpont, H. Coherent anti-stokes Raman scattering in Raman lasers and Raman wavelength converters. Laser Photonics Rev.4, 656–670 (2010).
Christopher, P., Xin, H. & Linic, S. Visible-light-enhanced catalytic oxidation reactions on plasmonic silver nanostructures. Nature Chemistry 3, 467–472 (2011).
Baffou, G. & Quidant, R. Thermo-plasmonics: using metallic nanostructures as nano-sources of heat. Laser & Photonics Reviews 7(2), 171–187 (2013).
Cao, L., Barsic, D.N., Guichard, A.R. & Brongersma M.L. Plasmon-Assisted Local Temperature Control to Pattern Individual Semiconductor Nanowires and Carbon Nanotubes. Nano Letters 7(11), 3523–3527 (2007).
Link S., El-Sayed M.A.; Shape and size dependence of radiative, non-radiative and photothermal properties of gold nanocrystals ; International Reviews in Physical Chemistry 19 (3), 409-453 (2000).
Oldenburg S.J., Averitt R.D., Westcott S.L., Halas N.J.; Nanoengineering of Optical Resonances; Chemical Physics Letters 288, 243-247 (1998).
Bardhan R., Mukherjee S., Halas N.J.; Nanosphere-in-a-nanoshell: A simple nanomatryushka; Journal of Physical Chemistry C 114, 7378-7383 (2010).
Hao F., Nordlander P., Maier S.A. et.al; Tunability of Subradiant Dipolar and Fano-Type Plasmon Resonances in Metallic Ring/Disk Cavities: Implications for Nanoscale Optical Sensing; ACS Nano 3 (3), 643-652 (2009).
Cognet L., Tardin C., Boyer D., Choquet D., Tamarat P., Lounis B.; Single metallic nanoparticle imaging for protein detection in cells; PNAS 100 (20); 11350-11355 (2003).
Ayala-Ozorco C., Urban C., Joshi A. et.al; Au Nanomatryoshkas as Efficient Near-Infrared Photothermal Transducers for Cancer Treatment: Benchmarking against Nanoshells; ACS Nano 8 (6), 6372-6381 (2014).
Baffou G., Quidant R.; Thermo-plasmonics: using metallic nanostructures as nano-sources of heat; Laser and Photonics Reviews 7(2), 171-187 (2013).
Cao L., Barsic D.N., Guichard A.R., Mark L. Brongersma M.L.; Plasmon-Assisted Local Temperature Control to Pattern Individual Semiconductor Nanowires and Carbon Nanotubes; Nano Letters 7 (11), 3523–3527 (2007).
Boyd D.A., Greengard L.,Brongersma M., El-Naggar M.Y., Goodwin D.G.; Plasmon-Assisted Chemical Vapor Deposition; Nanoletters 6 (11), 2592-2597 (2006).
Adleman J.R., Boyd D.A., Goodwin D.G., Psaltis D.; Heterogeneous catalysis mediated by plasmon heating; Nano Letters 9 (12), 4417–4423 (2009).
Fasciani C., BuenoAlejo C.J., Scaiano J.C. et.al; High-Temperature Organic Reactions at Room Temperature Using Plasmon Excitation: Decomposition of Dicumyl Peroxide; Organic Letters 13 (2), 204-207 (2011).
Haas K.M., Lear B.J. ; Degradation of polypropylene carbonate through plasmonic heating; Nanoscale 5, 5247-5251 (2013).